## Tekspenuh

(1)

ri, 1 OP% -k rý f': -" it. 11.31 ýý 1'- '"^'

": üi". a 3-t w. ýý b;.,.. -

;" *ii-.

v ý ýü

+15.. ý

I... .;,. ,ý :t ra +ý k 'i

### As

ýyt ýs .:: t'vr r ýýýýý,

"eýý

### olm-

(2)

Progress Report Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

Pl

### Thabiso Frans Matome

A project dissertation submitted to the Civil Engineering Programme

### January 2010

Thabiso Frans Matorne 8820

(3)

Progress Report Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

### TIIAI3ISO FRANS MATOME

ii Thabiso Frans Matome

8820

(4)

Progress Report Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

### ABSTRACT

In the design of I-lot Mix Asphalt (I IMA) the aggregate gradation is one of the important factors that have to be considered in pavement design and ultimately, in the constriction, because it accounts for the overall strength of asphalt in terns of resisting pennanent deformation such as pitting. The pui-hosc of' this project is to implement the aggregate gradation analysis to a mix, which follows the standard of Malaysia in accordance with the Jabatan Keija Raya (JKR) standard specification for road works of Malaysia, using the Bailey method of gradation which follows a design and analysis procedure that includes an examination of aggregate packing and aggregate interlock, blending aggregates by volume, a new understanding of coarse and fine aggregate, and analysis of the resulting gradation.

'l'he idea was to analyze and compare, based on the Marshall Mix design factors and the I lamburg \Vhcel track test, a hot-mix asphalt (I IMA) constructed using aggregates with it gradation limit that is in accordance with JKR and an I IMA constructed using aggregates that are optimized by the Bailey method which uses aggregate packing concepts to analyze the combined gradation and relate the packing characteristics to the mixture volumetric properties and compaction characteristics. During the course of the research, the findings gave us a basis in which to analyze whether this method can he adopted and also if it will he useful and/or beneficial to the Malaysian pavement design industry.

What the lindings yielded was that the I IMA designed following the JKR standards i. e.

ACVV 20 wearing course, according to the bailey method, is as follows:

" 'fhe mix yaS SusceptibIC to segregation

" 1las a possibility of tenderizing

" May be difficult to compact

### So the bailey method was able to yield it new and better performing I IMA blend.

Thabiso Frans Ma tome 8820

(5)

Progress Report

Aggregate Grading Analysis Using The Bailey Method ofGradao n Seleco n INrveaýItl

I IA"YýIIk I

I. 1 IPt INA'

### The author wishes to express the deepest gratitude and appreciation to the project supervisor Assoc. Prof Dr. Madzlan Napiah for his motivation, generosity and patient supervision, comments, valuable suggestions and freedom to wholly undertake this projcct/study on my own.

Appreciation is also extended to PG student Yasreen Gasm Elkhalig on her input based on her thesis titled The Performance of Conventional and Polymer Modified Bituminous Mixture Containing Different Types of Sand as Fine Aggregate " and also the lab technician Mr. Iskandar from highway engineering laboratory for their guidance and advice in conducting the research and also to my colleagues for their support and collaboration

iv Thabiso Frans Matome

8820

(6)

Progress Report Aggregate Grading Analysis Using The Bailey Method of Grodoo n Seleco n

### CHAPTER 1: INTRODUCTION

1.1 Background of Study

### .

12 Problem Statement

### 1.3 Objectives and Scope of Study CHAPTER 2:

and rutting resistance Theory .

2.1.3 Effect of aggregate grading on I IMA properties.

2.2 Bailey Method Principles .

iii

### REFERENCES APPENDICES

3.1 Elements E)etcniiination. Sample Preparation

and 'I csting .

### RESULTS & DISCUSSION

4.1 Aggregate and Binder Tests.

### 5.1 Conclusion 36

11 Table AI- Recommended Ranges of Aggregate Ratios

Table A2 - Control Sieves for various Asphalt Mixes.

III Table A4 - Fine Graded Mixture Control Sieves

..

### 37 38

I Figure 1- Example ofbreak between coarse

### 40

V Thabiso Frans Matome

8820

(7)

Progress Report Aggregate Grading Analysis Using The Bailey Method ofGrodao n Seleco n

### TABLE 4.1.9

List of Table

Minimum VMA recommended by asphalt institute The Factors affecting VMA on an LIMA

Superpavc standard Sieve Size

### Standard Penetration "Test

Particle Density and Water Absorption (Sand) Particle Density and Water Absorption (Granite)

Flakiness Index (Granite)

Combined gradation of the mix Design Bitumen Content

Combined Average Results from Marshall Tests (20 mm continuously graded Asphalt)

The new control sieves for the 20 mm LAMAS aggregate

List of Figures

### FIGURI: 2.1.1 FIGURI: 2.12 FIGURIý, 2.1.3 FIGURE 4.1.1 FIGURF. 4.1.2 FIGURI: 4.1.3 FIGURF 4.1.4 FIGURE 4.1.5 FIGURI: 4.1.6 FIGURE 4.1.7

Thabiso Frans Motome 8820

### Voids Filled Willi vs. Asphalt Cement Content curve

VI

(8)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

### The Bailey method, based on experience, is a practical tool successfully utilized for developing and analyzing hot mix asphalt in the laboratory and in the field. It also provides a good starting point for mix design and is an invaluable aid when making adjustments at the plant to improve air voids, Voids in mineral aggregates (VMA) and the overall workability of the mix, whether using Marshall or Superpave (Pine 2005).

This method, The Bailey method, mainly focuses on aggregate packing. The determination of which particles/aggregates form the coarse fraction of the aggregate structure, meaning which particles/aggregates form the voids, and which ones fit into the voids created by the coarse fraction within the overall stnicture. This has to be known in order to understand the aggregate packing characteristics of the stnicture.

An evaluation of the individual aggregates and the combined aggregate blend by volume as well as by weight is also included in the method. The latter is done in order to better understand which fraction, whether coarse or tine, is controlling the overall aggregate structure.

1

Thobiso Frans Motome 8820

(9)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Gradao n Scleco n

### 1.3 Objective and Scope of Study

The objectives of this study are to:

### ": " Incorporate an analytical gradation design and evaluation method into the Marshal mix design procedure

Analyze, theoretically, the compaction and performance characteristics of the resulting hot mix asphalt mixture(s).

### ": " Design a new blend and compare the latter mix (Bailey method) to the JKR standard IIMA.

2

Thobiso Frans Matome 8820

(10)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

The Bailey method of aggregate gradation and evaluation will be used to design and evaluate the aggregate strictures for the mixture(s) in the study. The compaction characteristics of the mixtures will be analyzed and the perfonnance of the designed

mixtures will be evaluated using both simulative and fundamental laboratory tests.

Gradation parameters will be used to analyze the effect of gradation on compaction and perfonnance properties of asphalt mixtures. The aggregate types that will he used will be the ones commonly used in Malaysia i. e. granite and, three aggregate structures (coarse, medium, and fine) will be designed using the Bailey method of aggregate gradation evaluation. The asphalt mixtures will have a certain NMPS mixtures and will be designed for particular volume of traffic. A certain perfonnance grade, based on the JKR, binder will be used for the mixtures. Laboratory tests, namely sieve analysis, Marshall Tests, etc will be conducted, including the llamburg wheel tracking test.

3

Thabiso Frans Motome 8820

(11)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method ofGradao n Seleco n

### (2000)

VMA is the volume of inter-granular void space between the aggregate particles of a compacted paving mixture. It includes the air voids and the volume of the asphalt not absorbed into the aggregate. In other words, VMA describes the portion of space in a compacted asphalt pavement or specimen which is not occupied by the aggregate. VMA

is expressed as a percentage of the total volume of the mix. When aggregate particles are coated with asphalt binder, a portion of the asphalt binder is absorbed into the aggregate, whereas the remainder of the asphalt binder forms a film on the outside of the individual aggregate particles. Since the aggregate particles do not consolidate to fhrim a solid mass, air pockets also appear within the asphalt-aggregate mixture. Therefore, as Figure 2.1.1 illustrates, the four general components of IIMA are: aggregate, absorbed asphalt, asphalt not absorbed into the aggregate (effective asphalt), and air. Air and effective asphalt, when combined, are defined as VMA.

Air

V NIA

. Aggregate

_1ggi egate Particle f'olnine

### VMf\ is calculated according to the following relationship:

4

Thabiso Frans Matome 8820

(12)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

### Table 2.1.1 Minimum VN1A recommended by asphalt institute

I NI VI RNiI It", )it PLIRUNÄ)

Nominal \Iasiiniun Minimum VILA, percent

Particle Sizei'

imn üi.

Desitu Air Voids, percent 3

3.0 4.0 5.0

21.5 22.5

14.0

### 63 2.5 9.0 10.0 11.0

1- Standard Specification for Cue Clcth Sieves for Testing purposes.. ASTM EI I (AASHTO M92) 2- The nominal maximum particle size is one size larger than the firs sieve to retain more than 10 pet cent 3- Interpolate ttunimuun voids in the nuneral agereaate (, "%IA) for design air void values between those listed.

Analysis of the contribution of VMA to pavement durability, it is important to understand the parameters of an IIMA that relate to the determination of VMA. Certain characteristics of' an HMA mixture and its components can change the VMA and film

thickness. These characteristics are summarized in Table 2.1.2

5

Thabiso Frans Matome 8820

(13)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodoo n Seleco n

### Table 2.1.2 The factors affecting VNIA on an 1IMA

UNIVfRSIT1 ffKfXllixa

üiRöhXS

Factor Effect on Vi\IA

### Aggregate Shape

More rounded aggiegates decrease VMA Aggregate Texture Smooth or polished aggregates decrease VNIA

Asphalt Absorption

asphalt

### absorption

results n1 lower effective asphalt

Dust Content

### Higher

dust contents Increase surface area, decrease

### film thickness,

and tend to lower

### Baghouse Increased fines and dust increase surface area. decrease film Fines Generation of Dust thickness, and tend to lower VVIA

Plant Fl-«luction

### Higher plant production temperatures decrease asphalt binder Temperature viscosity, which results in more asphalt absorption. lower

effective asphalt

and

### lower VMA

Ternpelanu e of MIA Higher temperatures during paving create soft iuixtlues, lower during Paving air voids, and lower V IA

Halllilin Tii11e

### lower

effective asphalt content and

### lower V NIA

More steps in aggregate

### handling

increases potential for

Aggregate Handling

aggregate

resulting in an increase in fines,

### and

lower V\IA

Alatellal PI-o/x'r-ties

The extent to which an I IMA mixture can be compacted is related to aggregate gradation, aggregate surfäcc characteristics, amount of asphalt, and asphalt absorption by the aggregate. Aggregate gradation is the size distribution of the aggregate particles, including the amount of material passing the 75-mm sieve (dust content). Aggregate surtiicc characteristics include the shape, angularity, and surfäcc texture. Aggregate absorption of asphalt binder is dependent on the aggregate porosity, and pore size, as well as the viscosity of the asphalt binder.

6

Thabiso Frans Matome 8820

(14)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

When selecting an aggregate for an I IMA mixture, the initial focus is on the aggregate gradation. Two factors relating to aggregate gradation having the most in ýuence on VMA are density, or the ability of the aggregate particles to pack together, and the aggregate surface area.

Density

Figure 2.1 illustrates a 0.45 power plot of an aggregate gradation developed by the Federal Highway Administration (FHWA). It is used to estimate how densely a given aggregate mixture will compact. It consists of the particle size raised to the 0.45 power on the x-axis and the percent passing each sieve size plotted on an arithmetic y-axis. A

line drawn from the origin of this plot through the nominal maximum aggregate size is estimated as the maximum density line for any given aggregate (The nominal maximum aggregate size is defined as the first sieve to retain between 0 and 10% of the aggregate).

An aggregate having a gradation that produces a straight line on a 0.45 power gradation graph will have the maximum achievable density, and subsequently the lowest air void content and the lowest VMA in an HMA mixture. Deviating from the maximum density line in either the fine or the coarse direction will tend to increase the VMA of the compacted mixture shown in Figure 2.1.2. Ilowever, note that significant confusion exists concerning different methods used to draw aggregate gradation "maximum"

density lines. Closely related to maximum density lines, and also in debate, is the definition of nominal aggregate maximum size. For the purposes of this paper, the definitions used For the maximum density line and the aggregate nominal maximum size are stated above.

7

IINIVIRSITI III: N OU%: 1 fti RUNZ

Thabiso Frans Motorre 8820

(15)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

zJ1 7 rA cu

O1

### Figure 2.1.2 Maximum density line related to VMA

The "distance" as the absolute value of the difference in percent passing between the actual gradation and the maximum density line at a given sieve size. This value characterizes the actual deviation from the maximum density line. Increasing the sum of the distances between a gradation and the maximum density line will tend to increase the VMA. The distances for the 2.36-nun and smaller sieve sizes had the greatest effect on the VMA of the compacted mixture. The percent passing the 4.75-nmi, 2.36-mm, 1. I8-mm, 0.600-mm, 0.300-mm, 0.150-mm, and 0.075-mnl sieves were the most practical predictive variables for VMA. This attempts to correlate "distance" to VMA.

These two variables did not correlate well due to the many other factors that affect VMA. Consequently, the only way to he certain of the VMA of a mix is to produce a sample and measure the parameters from which VMA is calculated.

### 2.1.2 The bailey method of aggregate gradation selection and rutting resistance as described by Promwell ct al. (2005)

In a study conducted at the University of Arkansas, which was an "Investigation of the use of the Bailey method of aggregate gradation selection for asphalt mix design in Arkansas" it was found that developing/creating Superpave mix designs using the Bailey Method for the selection of aggregate gradation proved to be more of a challenge than was expected

. Difficulty was encountered in creating aggregate blends with favourable Bailey Method parameters using the current gradations of existing aggregate

8

UNIYIRIITI it I: NCIZ0C: 1 Pt 11lÖWA-3

Thobiso Frans Matome 8820

(16)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

stockpiles Furthermore, in the process of adjusting the trial aggregate blends to achieve the specified volumetric property limits, the Bailey Method parameters commonly had to be adjusted to the limits of or slightly out of their recommended ranges. Furthermore, in terms of performance, the Bailey Method may improve pitting resistance more consistently and appreciably if ideal Bailey Method parameters (particularly the DUW) are met in the aggregate blends. IIowever, more research is required to conclusively determine if this is the case. When altering the mixture volumetrics, the methods outlined in the Bailey Method procedure for attaining the desired mixture volumetrics appear to be very effective based on the experience in this research project. In every instance where the outlined methods were utilized to adjust the VMA of the mix, the VMA changed in the expected direction. Based on the results of this research project, it appears that the Bailey Method of aggregate gradation selection may provide some degree of improvement to the pitting resistance of Superpave mixes designed with aggregates as they exist in stockpiles common in Arkansas

2.1.3 Effect of aggregate grading on l IMA properties adopted from Wald (2002)

Gradation is perhaps the most important property of an aggregate because it affects almost all the important properties of PIMA, including stiffness. stability, durability, permeability, workability, fatigue resistance, frictional resistance, and resistance to moisture damage. The mixture volumetric properties including asphalt content, VMA, and VFA have been identified as important parameters for durability and performance.

Ilowcver, (lie VMA is considered the most important parameter and is used in the Supcrpavc mixture design specifications to eliminate use of potentially poor-performing mixtures.

The Supcrpave mix design procedure controls the gradation of aggregate with a set of several specifications. The specifications were not developed from the results of actual,

9

t1NIVtRSIiI IEI: N(I111(; I

il 1 RUNAS

Thabiso Frans Matome 8820

(17)

Dissertao n Aggregate Grading Analysis Using The Bailey Method ofGradao n Seleco n

## 1 12.5 9.5 1/2 in 3/8 in

1

### 0.075 #200

Superpave asphalt mixtures are always classiticd as one of the following sizes: 37 .5 nun, 25.0 nun, 19.0 nun, 12.5 mm, 9 .5 nun, or 4.75 nun. This classification, referred to as the Nominal Maximum Aggregate Size (NMAS) of the mix, is defined as being one sieve size larger than the first sieve that retains more than 10 percent of the aggregate blend.

The 0.45 power chart is a plot with an x-axis consisting of the standard sieve sizes raised to the 0

. 45 power and a y-axis consisting of the percent of the aggregate blend passing the standard sieves. The x-axis has a minimum value of zero and a maximum value of

10

ý VnTRNn

PIfP. IY: Ati

Thabiso Frans Matome 8820

(18)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

the maximum aggregate size of the mix. Thus, the range of the x-axis of the 0 . 45 power chart varies with LAMAS of the Superpave mix. The y-axis always ranges from 0 to 100 percent with 100 percent being at the point of' intersection with the x-axis. The Superpave 0

. 45 power chart contains a "maximum density line" that nets from the origin (Omm, 100 percent passing) to the maximum x and y values (MAS 0 . 45,0 percent passing). This maximum density line on the 0 . 45 power chart is based on the findings of several studies.

### further investigated Nijboers findings and found that gradations similar to those used in actual road construction had the densest packing configuration when plotted at the same 0.45 slope on a log scale plot. Based on their findings, Goode and Lufsey developed what has become known as the 0 . 45 power chart. In 1992,1-tuber and Shulcr discovered that a gradation plotted on a0 . 45 power chart produced the densest packing when it created a straight line from the origin to the maximum x and y values on the 0 . 45 power chart (MAS, 100 percent passing). This line is included on the Supcrpave 0 . 45 power chart and is referred to as the maxims m density line as it theoretically represents the densest possible aggregate gradation.

A set of control points is also included on the Superpave 0.45 power chart. These points delineate the allowable ranges through which the aggregate gradations may pass. The control points are located at the sieve sizes coinciding with the MAS and the LAMAS of the mix, at the 2 . 36 nun sieve and at the 0.075 mm sieve. The control points assure that the NMAS and MAS definitions are met to ensure that the mixtures are relatively dense graded, and dictate the amount of fine material that an aggregate blend may contain. The limits set by the control points vary depending on the NMAS of the mixture. An example 0 . 45 power chart for a 12 .5 mm NMAS Supcrpave mix is shown in Figure 2.1.3

11

VNR'I RSI il ItKM%[k. l Pf FRO NAf

Thabiso Frans Matome 8820

(19)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

100

90

70

### I

t \ili4ý': I II 1'L I RUNAS

Conlrol Polnt< '

### /

Maxlmum Demwty Line

Conb-d Point

/ . ý ý "

. /

/ /

Control Points '"1

60

50

40

30

20

10

0 ý

I-

0

0

0

Sieve Slzt (mm)

N

### ý Figure 2.1.3 Superpave "0.45 1)o-,,., er chart" for a 12.5 mm WAS mix

The Superpave mix design procedure specifies that aggregate gradations must pass through the control points of the 0 . 45 power chart for the respective LAMAS of the asphalt mixture. Beyond this, no guidance is offered to mix designers on choosing the specific aggregate gradations for a Superpave mix. Figure 2 .1 demonstrates the open- endedness of the specification for choosing

the aggregate gradation . Mix designers are left to rely on experience and rules of thumb about the shape and location of the gradation curve when choosing the gradation of the aggregate blend. A specific procedure for choosing a proper aggregate gradation is desirable so that the mix design procedure will become more standardized and performance of the mixes may be optimized.

12

0 ý

Thabiso Frans Matome 8820

(20)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

### According to Jones (2006), the Four Main Principles of the Bailey Method are as follows s:

Principle I

Provides an entirely new definition of what is coarse and fine, and how to determine the volume of each:

### :" What coarse particles create voids and which ones fill them?

o The Bailey Method utilizes the Nominal Maximum A, ggregate Size (NMAS) to estimate the void size within the coarse fraction. The definition of NMAS is - the first sieve larger than the first sieve to retain more than 10% by weight. From this, a determination of the break between the coarse and Inne fractions can be done, which is defined as the Primary Control Sieve (PCS).

### o If the majority (>50.0%) of its gradation is retained above the PCS of the combined blend, then it will be treated as a coarse aggregates CA. If the

13

VN IVI RNf1 lik. ýaxixa f11RONA)

Thobiso Frans Matomc 8820

(21)

Dissertao n Aggregote Grading Analysis Using The Bailey Method of Gradoo n Seleco n

Principle 2

### I low does the fine fraction pack?

V To what extent is the coarse fraction compactable or susceptible to segregation?

Principle 3

### The bailey's principles must be monitored for changes because they are interactive, meaning when one is altered then the remaining 3 will also change. Thus all of_ the four principles should be reviewed if'a gradation changes.

Furthermore, the bailey method only mainly focuses if not limited to aggregate packing which is a major factor for the aggregate skeleton structure, this skeleton stnicture contributes to nit resistance strength but this is influenced by:

### ": Particle (aggregate) characteristics.

14

". i'. I Rm II II1. MNýk. I 1'l I RO'tiAl

Thabiso Frons Matome 8820

(22)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

### This in turn influences the VMA, Density and workability of tlic whole stricture thus it is connected to a number of variables.

15

I SNfF; 1111 IIAIxHIka PI 1ltl)NA1

Thabiso Frans Matome 8820

(23)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

### 3.1 Elements Determination, Sample Preparation and Testing

The objectives of this study are to sample, test, and analyze the aggregate source using the JKR standards for road works and also using the Bailey Method then to do a full Marshal mix on the I-IMA constructed using the JKR standards and repeat the inix design on the Bailey method optimized mix and ultimately compare the performance between the two mixes. The methodology used to accomplish these objectives will consist of the following tasks:

L Determination of the loose unit weight (LUW) and the dry rodded unit weight (RUW) and specific gravity properties of the individual fractionations/aggregate stockpile as per AASI ITO T 19.

### 11. Adjust as necessary to obtain desired volumetric properties.

16

UNIYUUITI 7I KNCM(K: 1 fl 1 RÜNÄi

Thobiso Frans Matome 8820

(24)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

12. Detennination of a suitable binder content for use in an asphalt mix as per (asphalt institute: Manual series no. 2) and in accordance with JKR 4.2.4.3 - (a)

### 15. Make recommendations for implementation of the Bailey design blend process and Bailey criteria.

17

Thabiso Frans Matome 8820

(25)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

### JKR 4.2.4.2 (c):

Bituminous binder for asphaltic concrete shall be penetration graded bitumen of 80-100 grade confirming to M. S. 124.

Table 4.1. I: Standard Penetration Test

tNIt7 Ri1T1 ll/acNika I'I IFI'ti

Detcrminatio n1

### 13 86 86 84

18

Thobiso Frans Matome 8820

(26)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

### Table 4.1.2: Particle Density and Water Absorption (Sand)

1.7\'IKfIil II Ar: UI[X, 1 1'F. 1R07dAl

### 1 2

Mass of saturated surface-dry sample in air

with water B

(g)

### C

Mass of oven-dry sample in air

Particle

on an [)

basis

### density on a A- (B - C) 2.56 2.56 2.560

19

Thabiso From Ma tome 8820

(27)

Dissertoo n

Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n I '. It'If; ýIII I IArwHix, l 1'i 1 ü0! iA1

saturated and surface-dried basis

### mass)

Particle Density and IVatcr Adsoipption (Granite) JKR 4.2.4.2 (a):

iv. The water absorption when tested in accordance with M. S. 30 shall be not more than 2%;

Table 4.1.3: Particle Density and Water Absorption (Granite)

### 1 2

Mass of saturated surface-dry sample in air

(g

### 0 1556 1562

Mass of oven-dry sample in air

### 1)

20

Thabiso Frans Matome 8820

(28)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Scleco n Ihlý'IF%III

11LhcXx; i 19 9 kimn%

### basis

Particle density on a

basis

Water

### (% of dry D

mass)

Flakiness Inclcv (Granite) JKR 4.2.4.2 (c):

### iv. The flakiness index when tested in accordance with M. S. 30 shall be not more than 25;

21

Thabiso Frons Matome 8820

(29)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

Table 4.1.4: Flakiness Index (Granite)

1`. IYI FI11

IIAhtAIK, I

i'I 1 N1ý1A1

### Retained (g) Passing (0%) tested, M2 (g)

gauge (g) gauge (g)

'T'otal

### Table 4.1.4: Flakiness Index (Granite)

`'l!

1 Yukiºtc. cslnclcr =` x1000, /o

### = 7.85%

22

Thobrso Frons Matome 8820

(30)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

### Sieve Analysis

According to the JKR standards, a mix gradation should follow or be within the limits of the table below

Table 4.1.5: Gradation Limit for Asphaltic Concrete adopted from JKR standards Clause 4.2.4.2

Mix Type Wearin Course Binder Course

Mix ACW 20 ACB 28

Desi nation

B. S Sieve % Passin by weig ht

37.5 mm 1 00

28.0 mm 10 0 80 - 100

20.0 mm 76 - 100 72 - 93

14.0 mm 64 - 89 S8 - 82

10.0 mm 56 - 81 50 - 75

5.0 mm 46 - 71 36 - 58

3.35 mm 32 - 58 30 - 52

1.18 mm 20 - 42 18 - 38

425 um 12 - 28 11 - 25

150 um 6- 16 5 - 14

77 l: I,

### i

8 3 - ES

23

l'. 'ý I\I{. 11 11 IIAtiýrilk, l Pl1RONAi

Thabiso Frons Motome 8820

(31)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Gradpo n Seleco n

### 'Table 4.1.6: Combined gradation of the mix

% passing

sieve size coarse fine filler %assin min max

28 100 100 100 100 100 100

20 99.4 100 100 99.75 76 100

14 51.45 100 100 79.61 64 89

5 0.1 100 100 58.04 46 71

3.35 0 98.6 100 57.3 32 58

1.18 0 65.2 100 40.6 20 42

0.425 0 18.6 100 17.3 12 28

0.15 0 1.4 94 8.22 6 16

0.075 0 1.4 ýý,

### C N

Vf ý Q D

120 100 80 60 40 20 0

0.1 1 10

sieve size

LAMAS

PCs scs

### i*

tMin --*-Max

-- result

The resulting gradation curve is well within the limit of the JKR standard and follows similar regime as a dense to open graded mixes which are suitable for all pavement layers and Ihr all traffic conditions. They work well for structural, friction, levelling and patching needs.

24

Nlt9 A'I I!

It), NU1(h; l PI I iRhNA)

Thobiso Frans Motome 8820

(32)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

Binder Content

the design

content will

range given

### The following are the results From the Marshall tests.

25

t! NIYI RSITI Ii ÄfJ()lllC. l ff I Rl)NÄ3

Thobiso Frons Matome 8820

(33)

Dissertoo n Aggregate Grading Analysis Using The Boiley Method of Gradoo n Seleco n

Table 4.1.8: Combined Average Results from Marshall Tests (20 nmm LAMAS continuously graded Asphalt)

AV % VMA % VFA %

Bitumen ratio

%

Flow

(mm) flow 0.25mm

Stability (KN) SG

SG. KGI M3

11.2 18.8 40.8 3.5 1.100 4.400 6.4 2 265 2265

9.5 18.4 48.3 4 1.395 5.580 7.4 2.290 2290

8.1 18.1 55.6 4.5 1.670 6.680 7.8 2.309 2309

6.4 17.7 63.9 5 1.383 5.533 8.0 2.333 2333

5.1 17.7 70.9 5.5 1.940 7.760 7.7 2.347 2347

4.5 18.2 75.3 6 2.180 8.720 6.8 2.345 2345

3.8 18.6 79.7 6.5 2.480 9.920 6.2 2.346 2346

3.8 19.6 80.8 7 2.590 10.360 4.9 2.329 2329

density+asphalt content/80/river sand

CM ý

N N

2360 2340 2320 2300 2280 2260 2240 2220 2200

012345678

%asphalt cement

### Figure 4.1.2: Bulk Relative Density vs. Asphalt Cement Content curve

26

Thobiso Frons Ma tome 8820

(34)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodoo n Sclcco n

z Y -n

a

### ý w .ý

stability+asphalt content/80/river sand

012345 a' 78

%asphalt cement

### Figure 4.1.3: Marshall Stability vs. Asphalt Cement Content curve

3 000 2.500 2 000 ý

1 500 0

1.000 0.500 0000

Iow+asphalt content/80/river sand

02R6E

%asphalt content

### VMA = 100 - ((100 - AC Content) BRD/RDA)

27

Thabiso Frans Matome 8820

(35)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradau n Seleco n

ýu cu a, 21

zm

Co

c13 (b Q1

ý

20.0

19.0

-18.0

17.0

Figure 4.1.5: Voids in Mineral Aggregate vs. Asphalt Content curve

### ý 0 ý

L Q ý O

air voids+asphalt content/80/river sand 12.0

11.0 10.0 9.0 8.0 7.0 6.0 5.0 4.0 3.0 2.0 1.0 0.0

voids in mineral aggregate- asphalt content/80/river sand

012345678

%Asphalt cement

012345678

%Asphalt cement

### 28

Thabiso Frans Motome 8820

(36)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

### VFB = 100 (100 - VMA - voids)/ VMA

voids filled asphalt+asphalt content/80/river s and

100 90 80 70 U-60 50 40 30 20

012345678

%Asphalt cement

### CA LUW = 13537.7 kg CA RUW 1513.4 k,, FARUW=1682.5kg

29

Thabiso Frans Matome 8820

(37)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodoo n Seleco n

### Secondary Control Sieve (SCS) = 0.22 * PCS = 1.18 mm Tertiary Control Sieve (TCS) = 0.22 * SCS = 0.15 mm

The mix is fine graded because majority of the material passes the PCS. The coarse aggregate is divided into the coarse portion of the coarse aggregate and the fine portion of the coarse aggregate. The coarse portion of the coarse aggregate is referred to as

"plugger" sized particles because they are the larger particles in the coarse aggregate segment which can pack together relatively tightly. The fine portion of the coarse aggregate is referred to as "interceptor" sized particles. No particle within the fine portion of the coarse aggregate (interceptors) should be able to fit within the voids created by the coarse portion of the coarse aggregate (pluggers). Thus interceptor sized particles within the coarse aggregate spread out the pluggers in the coarse aggregate, preventing them from packing as tightly together and creating more void space. The ratio of the percent "interceptors" to the percent of "pluggers" in the coarse aggregate is defined as the CA ratio which is as follows.

### CA Ratio = 0.153 [segregation susceptibility]

As the CA ratio of an aggregate blend decreases below 1.0, fewer interceptors are available to limit the compaction of larger coarse aggregate particles, so compaction of the fine aggregate increases. At a CA ratio less than 0.40, the resulting asphalt mixture may become susceptible to segregation.

30

Thobiso Frans Mo tome 8820

(38)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodoo n Seleco n

### Similar to the FAQ ratio, it is desirable to have values in the ranee of 0.35 - 0.50 for the FA1 ratio, in order to prevent overfilling of the voids created by the coarse fraction of the fine portion of the fine aggregate .

Blending nfuggregutes

### For CA, the voids created in the LUW condition

31

t. tVI r. alI I RN1IIY, I 1'F. I RU. 'rA1

Thabiso Frans Motorre 8820

(39)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodoo n Seleco n

### CA = 57.5% * 0.1 %=0.06`%, FA in CA stockpile

32

Thabiso Frans Matome 8820

(40)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Grodao n Seleco n

### 0.075mm contribution from CA = 57.56% * 0% = 0%

0.075mºn contribution from FA = 42.44% * 1.4% = 0.59%

### Total 0.075mm from CA and FA = 0% + 0.59% = 0.59%

The percentage mineral filler (MF) needed to achieve the total material passing the 0.075mm sieve desired:

### Only the FA percentage is revised to account for MF being added FA = 42.44 - 926 = 33.18%

Final aggregate percentage by weight = ('A = 57.56

### FA = 33.18 MF = 9.26

33

, '. S\ I S'. 'ý III

PIfRVhAS

Thobiso Frans Ma tome 8820

(41)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method ofGradao n Seleco n

### Table 4.1.9: The new control sieves for the 20 nim NMAS aggregate

passing

sieve size coarse fine filler Blend min max

28 100 100 100 100 100 100

20 99.4 100 100 99.75 76 100

14 51.45 100 100 79.61 64 89

10 13.35 100 100 63.61 56 81

5 0.1 100 100 58.04 46 71

1.18 0 65.2 100 40.6 20 42

0.425 0 18.6 100 17.3 12 28

0.15 0 1.4 100 8.7 6 16

0.075 0 1.4 80 7.1 4 8

NMASNew

PCSNew SCSNew

### " Decrease the segregation susceptibility

Evaluation and adjustment of trial aggregate blends is a trial and error undertaking that ultimately will put the CA Ratio, FA(' Ratio and FA; Ratio in acceptable or recommended bailey method ranges whereby from this point the marshal mix design

34

". It-Ii'+Iil I1 F. *. ý ý! +ii. 1 I'FIHOVAi

Thabiso Frans Matome 8820

(42)

Dissertao n Aggregate Grading Analysis Using The Bailey Method of Gradao n Seleco n

### the user.

35

Thabiso Frans Motome 8820

(43)

Dissertoo n Aggregate Grading Analysis Using The Bailey Method of Gradoo n Seleco n

### More research should be undertaken to further validate the Bailey method by using wheel tracking test devices to confirm any improvements in nit resistance.

Also further research into the use of the Bailey Method to improve I-IMA rutting performance appears to be feasible at this point. And as other agencies and academic institutions investigate the use of the Bailey Method and gain experience with the use of this procedure, refinements will be made that enable to Bailey Method to more consistently and significantly improve the rutting performance of IIMA. If this does not turn out to be the case, then further research into the use of the Bailey Method may not be justified. On the other hand, research into the development of a simplified procedure to alter mixture volumetric properties may be well warranted. A systematic, rational approach to the modification of mixture volumetrics could provide a very valuable enhancement to the Superpave Volumetric Design Procedure. Such it procedure could utilize the principles of aggregate packing that are the basis of' the Bailey Method procedure.

36

Thabiso Frans Matome 8820

Updating...

## Rujukan

Tajuk-tajuk berkaitan :